EN380 Notes on Wood and Timber as a Marine Material
Wood has been used as a shipbuilding and offshore structure material since the earliest days of
each industry. The USS
and the Standard Oil Company’s California Rig #1 are both
examples of w
term presence in the industry. On the shipbuilding side, over 40,000
wooden ships and small craft were built for the US Navy in WWII. The last US Navy wooden
purchases were the YP’s in the ‘80’s and the Avenger
class minesweepers (Figure 1)
in the ‘90’s.
At 224 feet, the Avengers are the longest wooden hulls built for the Navy.
Figure 1: USS
class wooden minesweeper
Commissioned in 1994
Although it is unlikely that the Navy will ever again purchase wooden hulled vessels (m
because of high initial costs compared to composites), wood’s properties make it a viable material
for structural use in the Navy for many years to come. In EN380 we will briefly explore these
First is a description of the microscopic pr
operties. Wood consists mainly of hollow fiber cells (sort
of like short soda straws) made of lignin and cellulose (Figure 2). The lignin acts as an adhesive
holding the cells together. The cellulose is a fibrous material that is hygroscopic, or attracts w
like a sponge. (And just like a sponge, wood will swell when moist.) The lignin is very strong, so
much so that wood typically fails by crushing of the cellulose structure rather than failure of the
Figure 2: Wood microstructure
tt = tg =
transverse, rr = radial, wr = wood ray
Wood is typically grouped into two classes: hardwoods and softwoods, although unfortunately
there is no correlation between these terms and the wood’s surface hardness. Hardwoods have
broad leaves and small fiber (ce
ll) sizes (about 0.01” diameter and 0.05” length). Softwoods are
conifers (have cones) and large cell sizes (0.05” x 0.13”). Balsa and oak are hardwoods, Douglas
fir, pine and cedar are softwoods.
Continuing the soda straw analo
gy will explain wood’s directional properties. If a soda straw is
held in the hand and squeezed between two fingers, the straw’s wall crushes. This is the
direction of the wood and like the straw it is not very strong. If the straw is held between t
hands in the long direction and pulled or pushed, it is strong as long as it does not buckle. This is
longitudinal (axial) or with
direction of the wood and is its strongest direction. The
last property direction is the
tangential or hoop
direction. This direction can be visualized by the
pressure built up in a straw if one end is capped and the other is blown in to. If the straw splits (or
“checks”), it is a tangential failure, and this is typically the weakest of wood’s three directions.
radial direction is slightly stronger than the tangential direction due to the presence of wood “rays”
(wood fibers). Few species have rays in the tangential direction, but those that do are highly
preferred in marine construction due to the increased
splintering resistance. The most notable are
Sitka Spruce, Live Oak, and Black Locust. The last two are fairly rare. On an historical footnote,
the 1797 frigates were specified for Live Oak frames and planking. Due to a shortage, only two
were built using
Live Oak rather than the inferior White Oak. One of those was the
In material science, a material which has the same properties in all directions is
considered isotropic). One which has different properties in e
very direction is
. If it has the different properties in three perpendicular planes it is
(composites are orthotropic). If one of the planes has the same material properties in all
directions it is
is a single fiber in a resin). These terms are
important when using Hooke’s Law. Wood is technically anisotropic but is usually modeled as
transversely isotropic. Composites are technically orthotropic but are also modeled as
transversely isotropic. Analy
tically, wood and composites share many characteristics.
The three directional properties of wood vary widely, but in general, if a wood species has a
longitudinal strength of 100, its radial strength will be about 5
10 and its tangential strength about
10. Given the large difference in properties it is clear that making sure the load is arranged with
the grain is critical to a structure’s success! This is often not easy as most trees do not grow
perfectly straight and lumber mills do not usually cut lum
ber for maximum strength.
Figure 3 shows a typical log undergoing the milling process. Depending on what part of the log
the plank comes from it will have dramatically different properties when exposed to moisture. The
“A” plank is quartersawn (or vertica
VG). This cut goes through the tree’s center and
gives planks that are warp stable. (See Figure 4.) Another advantage to this cut is that it
minimizes the weakest hoop direction fibers. The major disadvantage is that if small trees are
ks of a useful width for marine construction will often include sapwood, the outer rings
that are rot prone. Plainsawed planks of low density woods like pine, fir and cedar will often warp
as much as a plank thickness. The bottom line is that for any struc
tural application exposed to
moisture, quartersawn heartwood is specified.
Figure 3: Quartersawed (A) and plainsawed (B) boards cut from a log. (From Ref. 2)
Figure 4: Distortion due to sawing location of planks from the log. (From Ref. 2)
Material properties of wood are generally given for the longitudinal direction and are presented for
standard moisture content of 12%
. Radial and tangential properties are occasionally given but
are usually estimated from the previously me
ntioned ratio’s. If given, then usually the tangential,
being lower, is given. “
”, where the moisture content is above 18%, generally has
strength properties about ½ of the dry wood properties. Wood can be “green” either because it
has not dried
sufficiently after harvesting, or because of exposure to water after construction. As
the structures designed by naval architects and ocean engineers are often in a wet environment,
it is also important that they understand what will be the equilibrium moi
sture content of the wood
in their designs! A piece of wood may increase its weight 30% when submerged! The equation for
moisture content is:
Table 1 shows the material properties for common woods used in ships and offshore struct
Tensile properties parallel to the grain are usually taken as equal to the compressive strength,
although they are typically higher.
western red cedar
all properties are for oven dry samples
Table 1: Mechanical Properties of Common Woods used
in the Marine Environment (from Refs. 1 & 2)
in the Marine Environment
Apart from recreational craft, wood is still commonly used in fishing vessels and other small
commercial vessels worldwide. Its natural buoyancy, abundancy, and ability to be worked with
simple tools lend itself to marine constru
ction in developing countries. It has significant
disadvantages for large commercial and naval applications however, including:
Low modulus of elasticity (~1/6
that of aluminum)
Low fire resistance
Susceptibility to biodegradation
In the US
Navy, wood is still specified for well
decks of amphibious ships and as a damage
control material. Figure 5 shows “4x4’s” (four inch square lumber) stored on DDG
species are White oak, Eastern pine and Douglas fir.
Figure 5: Damage Control M
aterial on USS
Structural Analysis Equations
Because wood is essentially
, equations governing stress and strain are
different from isotropic materials. The most accurate way to analyze a wood structure would be to
se the same methods as for composites. In the case of plywood this is especially true as it is a
wood laminate. The mechanics approach for plywood and composites uses the
assumption which assumes that stresses through
thickness are zero.
In general practice though, because lumber is typically used in plank form, one axis dominates
the properties and the stresses in the other two directions are assumed zero. Little additional
error is created in using the resulting
For example, in axial loading, the deflection is given by the familiar:
where P is the axial force, L is the length, A is the cross
sectional area and E is the Young’s
modulus of the axial direction.
In bending the deflection of
a straight beam of constant cross
where the bending and shear constants (k
) are based on the loading and boundary
conditions (see Table 2), W is the total beam load acting perpendicular to the beam neutral axis
L is the span, I is the moment of inertia, G is the shear modulus and A’ is a modified shear area.
for rectangular beams,
for circular beams
for rectangular beams,
for circular beams
Table 2: k
for beam deflection
Again, due to the beam assumption, stress formulas for wood are the same as those of isotropic
for axial loads, and
for bending, a
where k is 3/2 for rectangular cross
sections and 4/3 for circular cross
Typical lumber dimensions lead to the possibility of buckling under compressive loading. The
critical buckling stress is:
where r is the radius of gyration,
for a rectangular section with b as the
smaller dimension and,
for a circular section.
As wood will creep under long
term load it is customary to design to half t
he allowable deflection
Wood is relatively easy to join compared to other materials. And as with other materials, joining
can be broadly classified into two methods:
en the two are that bonded joints are typically 1 ½
3 times stronger, but take
longer to assemble and are regarded as permanent.
Due to fastener degradation, adhesive bonding is required for long
term, efficient joints in the
marine environment. Adhesiv
es transfer load from one member (called an adherend) to another,
through the adhesive. In most cases the load transfer is designed as a shear load, as adhesives
are typically much stronger in shear than in tension. Factors involved in adhesively bonded jo
Type of wood
All of the woods noted above can be glued, although teak, oak and lignumvitae all require
specialized methods for satisfactory results. Figure 6 shows ty
pical edge and axial joints and
Figure 7 shows corner joints.
Figure 6: Edge (A
tongue and groove) and
finger) Bonded Wood Joints
Figure 7: Corner Bonded Wood Joint
fastened joints in wood use a stag
gering variety of fasteners. (Just walk down an
aisle at Home Depot.) Marine joints however, rely primarily on two types: wood screws and bolts.
In general, screws are used for lightly loaded, watertight connections. Bolts are used for high
, but are significantly more difficult to make watertight. Thin planking on small craft is
occasionally fastened with copper rivets.
An important corrosion issue is the reaction of wood fasteners. Traditionally the way to avoid
fastener corrosion was to u
se wood trunnels (dowels). In the US the preferred trunnel material
was Black Locust. These are relatively low
strength however and silicon bronze and monel are
preferred. If cost is an issue stainless or galvanized steel is used, although service life is
If cost is no object then titanium can be used.
Control of Degradation
Under ideal conditions wood structures can survive for centuries. The primary reasons wood
structures fail include fungi, insects, bacteria and marine borers. In some cases
have been known to fail within a month of infestation.
Fungi (rot) requires moisture, oxygen and mild temperatures and is considered the largest source
of marine decay. To foster rotting the moisture content must be above the fiber satu
(30%), and the temperature must be between 50 and 90
F. The best prevention methods include
ventilation, reduction of leaks, and preservatives. Note that most preservatives are toxic and
make painting difficult.
Insect attack includes termite
s, beetles and carpenter ants. Rarely are marine structures infected
by insects. Some vessels stored out of the water, or along infested docks, have become infected,
and alongshore structures are susceptible.
Damage by marine borers is worldwide, and can
occur in seawater, brackish and even fresh
water. Attack can be rapid, with pilings destroyed in less than six months. The primary borers are
(shipworm) which can grow to lengths of four feet in ideal conditions, and various
In all cases preservation techniques attempt to either impregnate the wood with toxic chemicals
or provide an impregnable barrier. Preservatives include copper compounds and creosote tars.
The allowable (by EPA or OSHA) versions chan
ge frequently. The US Navy currently favors a
combination of epoxy/glass coatings and copper antifouling paint for vessels and concrete
coverings for stationary structures.
Plywood is a glued
up lamination of many layers of wood. Figure 8 shows t
ypical 3, 4, and 5
construction. Compared to lumber, plywood is more stable and uniform. It’s axial and transverse
properties are similar and it is available in wider widths. Its primary disadvantage is that it is not
easily formable. Compound curves (
bending about two axes) is not possible. If formed in
into a curved shape (such as a boat hull) it is commonly called “cold
Figure 8: Plywood construction.
The individual plies are held together with various glues. Exterior,
marine, and aircraft
plywood are required to use waterproof grade. The difference between the three grades are the
number of flaws in each ply, and the variation is quite wide. In general, the price is reflective of
the ply quality and wood species.
Many marine applications can use exterior
grade. Aircraft grade
is rarely justified except in weight critical structures, and even then may not be desirable as many
woods used in aircraft ply are not rot resistant.
1. Wood: A M
anual for it Use as a Shipbuilding Material
, 4 Volumes, Bureau of Ships,
Department of the Navy, 1957
2. The Encyclopedia of Wood, Revised Edition
, Sterling Publishing, New York, 1989 (Also called,
Wood Handbook: Wood as an Engineering Material
e US Government Printing Office)
What are the expected tangential, longitudinal and radial tensile strengths of white oak when
wet and dry?
You select a douglas fir “4x4”, whose actual dimensions are 10’2”x3.9”x3.8” and weighs 31
ds, 5 ounces. Is it wet or dry?
What is unique about lignumvitae?
Compare the specific (meaning per pound) stiffness, specific compressive strength and
specific flexural strength (ie strength/density) of sitka spruce, aluminum and steel. Which
e best in stiffness and strength for weight critical applications?
Why is wood a material of choice for controlling flooding and for minesweeper construction?
A 8’x8’x8’ compartment on your ship is flooded with seawater. Due to the worry of the deck
sing you decide to brace it with 4x4’s. What is your estimate of the load? Is this a
conservative engineering estimate? Why? How many 4x4’s would be required if they were
vertical? What is the possible problem with this arrangement? (Think multi
4x4’s would be needed if the supports were canted 45 degrees to the vertical?
Using the internet, locate a
wood preservative available today that would work in the